# 2D analysis of laminated composite and sandwich plates using a new fifth-order plate theory

Livre

0
0
27
1 year ago
Preview
Full text

2D analysis of laminated composite and sandwich plates using a new

fifth-order plate theory

Abstract a*

In the present paper, a new fifth-order shear and normal deformation N. S. Naik a theory (FOSNDT) is developed for the bi-directional bending analysis of

A. S. Sayyad laminated composite and sandwich plates subjected to transverse loads. a

This theory considered the effects of both transverse shear and normal Department of Civil Engineering, SRES’s Sanjivani deformations. In-plane displacements use a polynomial shape function College of Engineering, Savitribai Phule Pune

expanded up to fifth-order in terms of the thickness coordinate to properly University, Kopargaon-423603, Maharashtra, India.

E-mail: nitin_adi59@rediffmail.com, account the effect of transverse shear deformation. Transverse attu_sayyad@yahoo.co.in displacement is the function of x, y and z- coordinates to account the effect of transverse normal deformations i.e. thickness stretching. Hence, the

• Corresponding author

present theory involves nine unknowns in the displacement field. The present theory does not require a problem dependent shear correction http://dx.doi.org/10.1590/1679-78254834 factor as it satisfies traction free boundary conditions at top and bottom surfaces of the plate. The governing differential equations and associated Received: January 18, 2018

In Revised Form: June 22, 2018 boundary conditions are obtained using the principle of virtual work. The

Accepted: July 31, 2018 plate is analysed for simply supported boundary conditions using Navier’s

Available Online: August 01, 2018 solution technique. To prove the efficiency of the present theory, the non- dimensional displacements and stresses obtained for laminated composite and sandwich plates are compared with existing exact elasticity solutions and other theories. It is observed from the comparision that the displacements and stresses obtained by the present theory are in excellent agreement with the results obtained by exact elasticity solutions compared to other higher-order plate theories available in the literature.

Keywords

2D analysis, fifth-order, shear deformation, normal deformation, shear correction factor, laminated, sandwich.

## 1 INTRODUCTION

Due to attractive structural properties like high strength-to-weight and high stiffness-to-weight ratios, the demand of composite materials is increased in many engineering industries such as mechanical engineering, marine engineering, civil engineering, aerospace engineering, etc. Therefore, accurate prediction of bending behaviour of the structures made of advanced composite materials is an important part of the analysis. One of the important steps to develop accurate analysis of composite plates is to select a proper structural theory for the problem.

The analyses of laminated composite plates have been based on one of the following approaches. 1) Equivalent single layer (ESL) theories 2) Layer wise theories and 3) Three dimensional elasticity theories. The fundamental objective in the development of elasticity solution is to obtain accurate results of global and local quantities. These solutions are serving as benchmark solution for approximate theories. Pagano (1970) and Zenkour (2007) have developed exact elasticity solutions for rectangular bidirectional composites and sandwich plates. Since three dimensional elasticity theories and layer wise theories are computationally difficult, equivalent single layer theories are widely used for the modeling and analysis of laminated composite thick plates. The ESL theories are those in which a heterogeneous laminate plate is treated as a statically equivalent single layer having a complex constitutive behaviour, reducing the 3D continuum problem to a 2D problem.

The simplest ESL laminate theory is the classical laminated plate theory (CLPT) of Kirchhoff (1850). But, when CLPT is applied to the analysis of composite plates it underpredicts the deflections and stresses, and overpredicts natural frequencies and critical buckling loads. This is due to neglect of transverse shear deformation. Therefore, CLPT is suitable for thin plate only. To overcome this drawback of CLPT, Mindlin (1951) has developed first order shear deformation theory (FSDT) which considers the linear variation of transverse shear deformation across the thickness of the plate. The FSDT shows constant variation of transverse shear stress through the thickness of the plate and required shear correction factor to properly account the strain energy due to shear deformation. These limitations of CLPT and FSDT leads to the development of higher order refined plate theories.

Several higher order refined plate theories are developed by various researchers which uses polynomial and non-polynomial type shape functions to properly account the effect of shear deformation (Polynomial: Ambartsumian, 1958; Reddy, 1984; Pandya and Kant, 1988; etc. Non-polynomial: Levy, 1877; Touratier, 1991; Soldatos, 1992; Karama et al., 2009; Mantari et al., 2012; Grover et al., 2013; Sayyad and Ghugal, 2017a etc.). One can refer recently published review articles by Sayyad and Ghugal (2015a, 2017b) for other refined beam and plate theories available in the literature. Chakrabarti and Sheikh (2005) have studied the bending response of sandwich plates with stiff laminated face using six noded triangular element having seven degrees of freedom at each node. Zhen and Wanji (2007) have presented a study of global-local higher order theories for laminated composite plates. Thai et al. (2012) have presented a novel finite element formulation for static, free vibration and buckling analyses of laminated composite plates. Thai and Choi (2013) have developed a simple first order shear deformation theory for laminated composite plates, the theory contains only four unknowns and having similarities with the CPT and Navier’s solution approach is used to obtain solution. Sayyad and Ghugal (2015b) have presented a four-variable trigonometric plate theory for thermoelastic bending analysis of laminated composite plates subjected to thermal load liner across the thickness.

In all the aforementioned refined plate theories, the effect of transverse normal deformation i.e. thickness stretching is neglected to minimize the unknown variables. But, according to recommendations of Kant and Swaminathan (2002) and Carrera (2005); the effects of both transverse shear and normal deformations plays important role to predict accurate structural behaviour of laminated composite thick plates. Few researchers have developed refined plate theories for the analysis of laminated composite plates considering both transverse shear and normal deformations such as Ghugal and Sayyad (2013), Sayyad and Ghugal (2013, 2014a, b, c), Neves et al. (2011, 2012), Zenkour (2013), Carrera (1999a, 1999b, 2002, 2003).

In this paper, a new quasi-3D polynomial type plate theory is developed for the bidirectional bending analysis of laminated composite and sandwich plates. The present theory does not require a problem dependent shear correction factor as it satisfies traction free boundary conditions at top and bottom surfaces of the plate. The governing differential equations and associated boundary conditions are obtained using the principle of virtual work. The plate is analysed for simply supported boundary conditions using Navier’s solution technique. To prove the efficiency of the present theory, the non-dimensional displacements and stresses obtained for laminated composite and sandwich plates and are compared with existing exact elasticity solutions and other theories. The important contributions in the present study are summarized as follows:

1) In the present study, a new higher-order shear and normal deformation theory is developed and applied for the bi-directional bending of laminated composite and sandwich plates subjected to transverse loadings.

2) Since the present theory is polynomial type, it is computationally simpler than non-polynomial type plate theories recently developed by

many researchers. 3) The present theory different from the existing theories since, it considers the effects of transverse shear and normal deformations which are essential to avoid delamination type failures. Many theories available in the literature including theory of Reddy (1984) have neglected effect of transverse normal deformation i.e. thickness stretching. 4) The present theory is strongly recommended for the analysis of laminated composite and sandwich plates, because it yields accurate prediction of displacements and stresses compared to existing non-polynomial type theories.

5) The most important feature of the present theory is it predicts accurate interlaminar shear stresses as compared to any other refined plate

theories available in the literature.

### 1.1 Modeling of the composite plate

For the present study, a cross-ply laminated composite plate made of orthotropic fibrous composite material having length in direction, ‘b’ in direction and thickness ‘ in direction is considered (see Fig. 1). The plate

‘a’ x y h’ z

is subjected to an out of plane load ( ) and the mid-plane is located at 0.

q x, y z= Figure 1: Layer numbering system of laminated composite plate.

## 2 FIFTH-ORDER SHEAR AND NORMAL DEFORMATION THEORY

A fifth-order shear and normal deformation theory is initially developed by authors for the cylindrical bending i.e. 1D analysis of laminated composite plates (Naik and Sayyad 2018). In this study, it is extended for the bi-directional bending analysis of laminated composite and sandwich plates.

### 2.1 Kinematics of the present theory (FOSNDT)

The displacement field of the present theory (FOSNDT) can be expressed as

3

5

     w z z

4

16       u x y z u x y z z  x y z  x y

( , , ) ( , ) x ( , ) x ( , ) 

2  

4 

 x h h

3

5    

3

5

     w 4 z 16 z

( , , )  ( , )     ( , )    ( , ) v x y z v x y z z x y z x y

y y



2  

4 

 y 3 h 5 h

   

2

4

    4 z 16 z

(1)        w x y z ( , , ) w x y ( , )

1 ( , ) x y 1 ( , ) x y   z   z

2

4

h h     where are the and -directional displacements respectively of any point on the plate; , and

u, v and w x, y z u v w

    , , , and

are the displacements of mid-plane in x, y and z -directions respectively; x x y y are rotations of the  normal to the mid-plane about y and x axes which account the effect of transverse shear deformation. and z  z repressent higher-order transverse cross-sectional deformation modes i.e. effect of transverse normal deformations. The normal and shear strains are obtained within the framework of linear theory of elasticity as follows.

2

3

5

        u w z  z 

4

16

x x

     

 z z z x 2  2   4 

    x x h x h x

3

5    

2

3

5

       

  v w z y z y

4

16

      

z z z

y    

2

2

4

    y y h y h y

3

5    

3

   z  z

8

64    

   z z z



2   4 

 h  h  

2

             u v w  y  y

o x x     z   f z   f z

2    

xy   1  

2

        y x x y y x y x    

      '   '

z z       

f z   f z  

xz x 1 x

2

     

 x   x 

        ' ' z z

       f z f z    

(2)

yz y 1 y

2       y y     where

       

/2 0 0 /2 0 0

are Poisson’s ratios; the subscripts 1, 2, 3 correspond to

x, y

,

z

directions of Cartesian coordinate systems, respectively.

The nine variationally consistent governing differential equations associated with the present theory are obtained using the principle of virtual work. The analytical form of the principle of virtual work stated in Eq. (6)



( , ) a b h a b x x y y z z xy xy xz xz yz yz h dz dy dx q x y w dy dx             

23

        

  

(6) where



is the variational operator. After introducing stress resultants, the Eq. (6) can be written in following form

1

2

1

32 , , , , ,      

31

1

12

 

,

44

23

, Q G 

55

 ,

66

, Q G 

13

  12 21 23 32 31 13 12 23 31

1   2             

(5) where

E 1 ,

E 2 and

E 3 are the Young’s moduli; G 12 , G 13 and G 23 are the shear moduli and

12

21

2

2

3

z x xz xz x a b z z z xz yz y yz yz y yz

1

2

2

1

1

2

2 0 0

,

Q Q x Q Q Q Q Q dydx q x y wdy dx x y y

   

       

  

 

        

   





(7)

   

      

1

2

1

2

2

2

2

2 2 0 0

2

1

xy xy xy xy a b s s b b x x x x x x y y y y s s s s b y y z z z z xy xy xy y y s s s s x x xz

       

u w v w N M M M N M x x x x y y u v w

M M Q Q N N M y y y x x y M M M M Q y x y x

            

    

           

      

  

         

  

1 E Q

33

23

lamina of laminated plate under bending can be written as

11

12

13

12

22

23

13

33

(3) The 3D constitutive equations for the k

44

55

66 k k k x x y y z z yz yz xz xz xy xy

Q Q Q Q Q Q Q Q Q Q Q Q

       

   

         

     

th

               

  3 12 21

4

5

2

4 ' '

1

2

1

2

2

2

               

4

4

16

4

16 , , 1 and

1

3

5 z z z z f z z f z z f z f z h h h h

           

  

                 

1 E Q

1 31 21 32

13 E

Q

  

 

 ,

  2 13 31

22

  

     

 

,

 

2 32 21 31

Q

   

 

,

 

 ,

 

  

     

    (4) where

ij Q

are the reduced elastic constants, (

x y z xy xz yz , , , , ,      

) are the stress components and (

x y z xy xz yz , , , , ,      

) are the strain components. The following relationships between the reduced elastic constants and the engineering elastic constants are used for the present study.

  1 23 32

11

1 E Q

 

 

 ,

 

1 21 31 23

12 E

Q

## 13 Q G

### 2.2 Governing equations and boundary conditions

where

    

2

66

66

6

2

:

2

xy y x x y x x z z y x

N N u v w w u A A B B C C x y x x y x y x x y x u v w

D D

I J A A B C x y x x x y x y x y y C D D x y y

   



2

 

            

           

             

           

   

  

2

6 y

x y



 

2

2

2

2

2

11

12

11

12

11

12

2

3

2

2

2

2

2

2

3

2

11

12

13

13

66

66

66

66

2

  (9)

2

3



2

66

66

2

:

2

y xy y x y x x z z y x

N N u v w w v A A B B C C y x x y y x y y x y y u v w

D D

I J A A B C x y y y y x y x x y x y C D x x y

   

    

  

2

           

           

              

            

   

  

2

66

2 y

D x

 

 

2

2

2

2

3

3

2

12

22

12

22

12

22

2

2

3

2

2

2

2

2

3

2

12

22

23

23

66

66

66

66

3

2

, , x y xy

M z h

4 /2

, , , ,

4

4

16 , , ,

3

3

5

16

5

h h h h b b x x y y x x y y h h h h h h h s s s x x y y x x h h h h s y y h

N dz N dz M z dz M z dz z z z M z dz M z dz M z dz h h h z

       

4 /2 /2 /2

             

 

         

                 

   

   

      

1

2

1

2 /2 /2 /2

3

5

2

4 /2 /2 /2 /2 /2

1

N N N

are the resultant in-plane forces,

, , b b b x y xy

M M M are the moment resultants analogus to classical

plate theory;

1

1

1

2

2

2 , , , , , s s s s s s x y xy x y xy

M M M M M M are the moment resultants due to transverse shear deformation effects;

2

2

1

2

1

2 , , , , , s s xz xz yz yz z z

Q Q Q Q Q Q are the transverse shear and transverse normal stress resultants.

1

1

2

2 /2 /2 /2 /2 /2 /2 /2 /2

/2 /2 /2

3

3

5

2

3

2

Q dz Q dz h h

4 /2 /2 /2

2

4

1

2

2

4 /2 /2

16 , 1 ,

4

16 1 , 1 .

h h xz xz h h h yz yz yz yz h h

z dz Q dz h z z

     

4

   

   

   

       

       

   

(8) The governing differential equations and associated boundary conditions for the present theory can be obtained by integrating Eq. (7) by parts; collecting the coefficients of , , , u v w

  

, , , , and x x y y z z

     

and equating them equal to zero, the following equations can be obtained

2

2

/2 /2

2

/2 /2 /2 /2

5

5

2

1

4

2 /2 /2

8

64 , , ,

4 , , ,

3

16

4 ,

1

h h s s z z z z h h h h h s b xy xy xy xy xy xy h h h h s xy xy xz xz h h

      

z z dz Q Q h h z

N dz M z dz M z dz h z z

M z dz Q h h

      

         

  

   

     

   

   

       

       

       

(10)

2 b 2 b 2 b

3

3

4

4

   M M    

M y xy u v w w

x

      

 w q B B A As

:

2

11 12 s

11

12

2

2

3

2

4

2

2

 x  y   x y  x   x y  x   x y

3

3

3

3

2

2

3

        

 y  y   u x x z z

 C  C  D  D  I  J  B

s 11 s 12 s 11 s 12 s

13 s

13

12

3

2

3

2

2

2

2

          x x y x x y x x x y

3

3

3

4

4

3

3

           v w w y y

x x

       B A A C C D D (11)

22 s 12 s 22 s 12 s

22 s

12 s

22

3

2

2

4

2

3

2

3

 y   x y  y   x y  y   x y  y

2

2

3

3

4

3

      

  u v w z z x

     

I J B B A C

s 23 s

23

2

66

2

66

4 s

66

2 s

66

2

2

2

2

2

2

2

 y  y   x y   x y   x y   x y

3

3

3

 

   y  y x

 C  D  D   q

2

2

2

s 66 s 66 s

66

2

2

2

      x y x y x y

S s

1

2

2

3

3

2

1

  M      

M xy u v w w

x x

1        

Q C C C C C

x : xz s s ss

11

12

11 12 111

2

3

2

2

 x  y  x   x y  x   x y  x

2

2

2

2

2

 

  y   y      u  v x z z

 C  C  C  I  J  C  C

ss ss ss ss ss 112 211 212 113 113

66

66

2

           x y x x y x x x y x y (12)

2

2

3

2

2

           w y y

x x z

        C C C C C C C 2 s ss ss ss ss sss x sss

66

1 66 166 266 266 155 155

2

2

2

  x y  y   x y  y   x y  x  

z

    C C

sss x sss 255 255

 x

S

2 s

2

2

3

3

2

2

 M      

M xy u v w w 

x

2 x

      

 Q D D D D C

:

11

12

11 12 211 x xz 2 s 3 s 2 ss

2

         x y x x y x x y x

2

2

2

2

2

 

 

       u  v

y y x z z

       C D D

I J D D

ss 212 ss 111 ss 112 ss 213 ss 213

66

66

2

2

          x y x x y x x y x y (13)

2

2

3

2

2

          w y y 

x x z

       D C C D D C  C

2

66

26 6 266 166 166 255 255 s 2 ss 2 ss ss 2 ss sss x sss

  x y  y   x y  y   x y  x  

z

    D D

sss 155 x sss 155

 x

S S

1

1

2

2

3

3

2        

M y M xy u v w w

1 x

        : Q C C C C C y yz

12 22 s

12 s

22 ss 112

2

2

3           y x x y y x y y x y

2

2

2

2

2             y y x z z u v

       C ss C ss C ss

I ss J ss C C

122 212 222 123 123

66

66

2

2

2          y x y y y y x y x

(14)

2

2

3

2

2    

       w y y x x z

       

## 2 C s C ss C ss C ss C ss C sss y C sss

66

16 6 166 266 266 144 144

2

2

2          x y x y x x y x y

  z

    C sss y C sss 244 244

 y S S

2

2

3

3

2

2

2

 M  M      

y xy 2 u v w w x        

: Q D D D D C

y yz

12 22 s

12 s

22 ss 212

2

2

3

          y x x y y x y y x y

2

2

2

2

2

 

  y   y      u  v x z z

 C  D  D  I  J  D  D

ss 222 ss 112 ss 122 ss 223 ss 223

66

66

2

2

2

         y x y y y y x y x (15)

2

2

3

2

       w y  y 

x z

      

## 2 D C D D C  C D 

s 66 ss

26 6 ss 166 ss 166 sss 244 y sss 244 sss 144 y

2

2

2

  x y  x   x y  x  y 

 z

  D

sss 144

 y

1

1

2

2 

     Q       Q yz S y xz x z x z

1         : Q C C C C C z z sss sss sss sss sss 155 155 255 255 144

2

2        x y x x x x y

2

2

2

2        

 y  u v w w z z

       C C C

I I

I I (16) sss 144 sss 244 sss 244

13 23 s 13 s

23

2

2

2

2        y y y x y x y

        y y x x

         I ss I ss I ss I ss I sss z I sss z

113 123 213 223 133 233     x y x y

2

2

2

2    

Q       Q yz S xz x z x z

2        : Q C C D D z z sss sss sss sss 255 255 155 155

2

2       x y x x x x

2

2

2          y  y  z z u v w

      

C C D D J J J (17)

sss 244 sss 244 sss 144 sss 144

13 23 s

13

2

2

2        y y y y x y x

2    

     w y y x x

          J s J ss J ss J ss J ss I sss z J sss z

23 113 123 213 223 233 133

2      y x y x y

The boundary conditions along edges are of the following form: Along the edges =0 and = ,

x x a

u  N either 0 or is prescribed

x

 v N either 0 or xy is prescribed

b

 w M either 0 or x is prescribed

 w

b

 either 0 or M is prescribed

xy

 x

s

1



 M

either 0 or is prescribed

x x

(18)

s

2



 M

either x 0 or x is prescribed

s

1



 M

either y 0 or xy is prescribed

s

2



 M

either 0 or is prescribed

y xy

1  

either 0 or Q is prescribed

z xz

2





either 0 or Q is prescribed

z xz

Along the edges y =0 and y = b ,

1

2

1

2 /2 /2 " "

1

1

2

1

2 /2 /2 /2 " " "

2

1

1

2 /2

1

  /2 /2 ' ' ' ' '

     

     

       

  



    

  

  

2

, , , , , , ( ) 1, , , ,

   

(20)

(21) Following Navier’s solution procedure, the solution to the displacement variables to satisfy the above boundary conditions can be expressesd in the following forms.

         

2 0, 0, 0, 0, 0, 0, 0, 0, 0, s s b x x z z y y y y u w M M M N    

1

At edges y= 0 and y=b;

         

2 0, 0, 0, 0, 0, 0, 0, 0, 0, s s b y y z z x x x x v w M M M N    

1

Assuming that the plate is simply supported in such a way that tangential displacement is not admisible while the normal displacement is admisible. Following are the boundary conditions which will be satisfied the Navier’s solution. At edges x= 0 and x=a ;

   

, , 1, , ( )

 

  

      

  

 

     

I Q f z z f z f z dz J J J Q f z z f z dz

I I I

f z f z f z dz D Q f z f z dz

h h ij sss ij ij h h h ij sij sss ij sss ij ij h h ij sij sss ij ij h

 

I J Q f z z f z f z f z dz C C Q

2

2

(17) can be obtained as

(19) The extension, bending, bending-extension, bending-twisting stiffnesses used in the governing equations (9)-

  

  

M

s y y z yz z yz

ribed either 0 or is prescribed either 0 or Q is prescribed either 0 or Q is prescribed

2

1



 

       

 

 

 

 

  

M y M M M

u N v N w M w

o xy y b y b xy s x xy s x xy s y y

either 0 or is prescribed either 0 or is prescribed either 0 or , is prescribed either 0 or is prescribed either 0 or is prescribed either 0 or is prescribed either 0 or is presc

1

               

  /2

I J Q f z z f z f z f z f z dz D D D

2

A B A Q z z dz C C C C

h ij ij sij ij h h ij sij ss ij ss ij ss ij ss ij ij h h ij sij ss ij ss ij ss ij ij h sss ij sss ij

, , , , 1, , , , ,

, , 1, , , , , , , , 1, , , , , ,

2

2 /2 1 ,

1

2

2

2

2 /2 /2 " "

1

2 /2 /2 " "

1

2

1

1

1

1

2

1

### 2.4 Analytical solutions Here, the analytical solutions of Eqs. (9)- (17) for laminated composite and sandwich plates are considered.

    u f f u mn 2 3  

  v f f v  mn 1 4 

   

  w f f w mn 1 3

   

   f f    xmn 2 3

x  

       f f

(22)   x  xmn 2 3 

  m  1,3,5. n  1,3,5.

   

 y  f f ymn 1 4

       

  y f f ymn 1 4

   



    

z f f zmn 1 3

   

 

  z f f

zmn 1 3

  where  m x    m x    n y    n y  

    f sin , f cos , f sin , f cos (23)

1

2

3

4

        a a b b         and the loading term q ( x,y ) is expanded as

 

q x y ,  q f f (24)

  mn 1 3

    m 1,3,5.. 1,3,5.. n

   

where u v w   , , , , , , , and are the unknowns to be determined. q is the coefficient of

mn mn mn xmn xmn ymn ymn zmn zmn mn  q q

Fourier series expansion and; m and n are the positive integers. For sinusoidal load, and m=n= 1.

mn Substitution of Eqs. (22)- (24) into governing Eqs. (9)-(17) leads to the following equation.

  u  K K K K K K K K K 

11

12

13

14

15

16

17

18 19 

 mn

  

 v   K K K K K K K K K mn

21

22

23

24

25

26

27

28

29

  

   w

K K K K K K K K K mn q

31

32

33

34

35

36

37

38

39 mn

  

  



K K K K K K K K K  xmn  

41

42

43

44

45

46

47

48 49 

     

  

K K K K K K K K K   xmn    (25)

51

52

53

54

55

56

57

58

59

      

K K K K K K K K K ymn

61

62

63

64

65

66

67

68

69

     

K K K K K K K K K 

71

72

73

74

75

76

77

78

79

ymn

   

   K K K K K K K K K



81

82

83

8

4

85

86

87

88

89

  zmn    

   

K K K K K K K K K

91

92

93

94

95

96

97

98

99    



zmn 

 

ij

where the elements of stiffness matrix [ K ] can be defined as below

2 2 2 2

s s s s s s s s s

66

3

2

2 2 2 3 3

36

12

22

66

2

3

2 , 2 ,

2

m m n m n C C C a a b a b m m n m n

11

K D D D a a b a b m n n m

K C C C a b b     

       

         

        

       

           

      

             

         

    

       

12

35

2 2

           

2

4

2

2

, , , , , ,

2 4 ,

s s s s

m n m n K D D K

I a b a b n

K J K K K K b m m n n m n

K A A A A a a b b a b K

    

     

2 3 3 2 2 2 2

         

       

      

              

                   

3 3 2 2 2 2

34

11

12

66

3

2

   

2 2 2 3 3 2 2

4

2 2 2 2 2 45 211 266 255

    

 

 

  

       

      

             

             

                      

 

2 2 2 2 111 166 155

2

2

I I K J J K K a b a b K K K K K

2 46 112 166

, ,

,

ss ss sss ss ss sss ss ss

m n C C C a b m n

K C C C a b m n m n

K C C a b a b  

     

       

       

       

             

      

K

37

41

12

22

66

2

3

2 2 2 2 2 2 2 2 2

38

13

23

39

13

23

14

K D D D a b b a b m n m n

2

2

2

2

42

24

43

34

44

, 2 , , , ,

, ,

s s s s s s s

n a b m n n m n

2

66

11

66 2 2 2 2

         

            

2 2 2 2

11

66

2

2

16

12

66

17

12

18

      

13

19

13

21

12

22

22

66

2

2

, , , , , m n

D a b m n m n m n m n

             

         

K

3

11

66

12

12

66

2

2 2 2 3 3 2 2

13

12

11

66

2

2 2 2 2 2

           

14

11

66

15

2

2

, , 2 , , m n m n m n

K A A K A A a b a b a b m n m m n

K B B B a b a a b m n

K C C K D a b      

      

         

         

K C C K D D a b a b a b a b m m n m

I K J K K K A A a a b a  

22

28

     

         

            

         

                 

                       

    

   

2 2 2 2 2 2

27

22

66

23

K C C b     

2

2

2

29

23

31

13

32

23 4 4 2 2 2 2 4 4 2 2 2 2

33

11

12

        

K C C K D D a b a b a b a b n

           

12

    

       

                 

                       

     

       

       

 

3 3 2 2 2 2

23

22

66

3

K B B B b a b a b m n m n m n m n

2

2

24

12

66

25

12

66 2 2

26

22

66

2

, 2 , , , n m n m n

              

47 212 266 48 113 155 49 113 255

78 88 155 144 133

84

48

85

58 2 2 2 2

86

68

87

2

83

2 2 2 2 2 89 255 244 233

91

19

92

29

93

39

38

       

49

n K K K K K K K K K K b n m n n

81

18

82

28

, , , , , , ,

, , ,

ss ss sss ss sss ss sss

K K K D D D K

       

I C b a b b n n

K J D K K K K b b

      

      

   

       

              

       

94

2

2

, , , , , , , and x x y y z z u v w      

,

sss sss sss

K K m n K D D J a b

 

    

           

(26) After knowing the values of unknown displacement variables

from Eq. (22), all the displacement and stress components within the laminated composite plate under consideration can be calculated using Eqs. (1) through (5). The evaluation of transverse shear stresses from the constitutive relations leads to the discontinuity at the inter face of two adjacent layers of a laminate and thus violates the equilibrium conditions. Hence, transverse shear stresses and

2

xz yz  

can be obtained by using equilibrium equations of theory of elasticity neglecting body forces stated in Eq. (27).

xy x xz xy y yz yz xz z x y z x y z x y z 

       

        

         

       

2

79 98 89, 2 2 2 2 99 155 144 133

2

sss sss sss sss sss sss

95

59

96

69

97

, , , , , , ,

, , , , , , ,

K K K K K K m n K K K K K C C

  

I a b m n

K C C

I K K K K K K K K a b K K K K K K

   

      

             

           

       

2 79 223 144

67 77 122 166 144, 78 223 244

51

D m n m n K C C a b a b m n m n m m

       

     

155 56 212 266 57 112 166 58 213 255 59 213 155

61

, , , ,

,

sss ss ss ss ss ss sss ss sss

K D D K

             

I C a b a b a a m m

K J D K a a

           

 

 

        

                     

               

           

      

2

15

52

25 2 2 2 2

53

35

54

45 55 111 166

2

        

, , , , ,

, ,

ss ss ss sss ss sss ss ss

m n m n K C C a b a b m m m m

K

I C K J C K K K K a a a a m n

K K K K K D D a b

         

                        

       

76

71

       

               

         

           

     

     

44

17

K J C b

72

27

73

37

74

47

75

57 2 2 2 2

      

I C b a b b n

16

56 2 2 2 2 66 122 166 144

62

26

63

36

64

46

65

2

K C C C K

2 2 2 2 2 67 222 266 144

68 123 144

2

2 69 123

2

, , , , , ,

, ,

ss ss sss ss ss sss ss sss ss sss

K K K K K K K K K n m K C C C b a n m n n

(27)

   , ,

The in-plane normal and shear stresses calculated from constitutive relations are substituted in

x y xy   ,

Eq. (27). The transverse stress stresses ( ) are evaluated by integrating Eq. (27) layerwise through the

xz yz thickness coordinate ( ). z

### 3.0 NUMERICAL RESULTS AND DISCUSSION

In this section, various numerical examples solved are described and discussed for the bending analysis of laminated composite and sandwich plates using the present theory. In the present study, different configurations of the laminates are used and a simply supported plate subjected to transverse sinusoidal loading is considerd. Results are obtained using the present FOSNDT in closed form using Navier’s solution technique for above geometry and loading. The accuracy of the solution is checked by comparing results obtained using the present theory (FOSNDT) with the other theories and the exact elasticity solution wherever available in the literature. The following sets of material properties are used in obtaining numerical results for the present study.

a) Isotropic

E               

E E E G G G G

1

2 3 210 GPa,

13

23 12 ,

12

32

31

0.3 (28)   2 1  

b) Transversely Isotropic

     0.04,  0.5,   0.06,  0.016,   

0.25 E E E G G G (29)

1

2

3

13

23

12

12

32

31

c) Fibrous Composite (Graphite-Epoxy)

E E G G G

1

3

12

13

23

 25,  1,   0.5,  0.2,      

0.25 (30)

12

13

23

E E E E E

2

2

2

2

2 For the validity of the present theory, following examples are solved for the numerical study.

2. Bi-directional bending of two-layer (0 /90 ) antisymmetric cross-ply laminated composite plates under sinusoidal loading.

3. Bi-directional bending of three-layer (0 /90 /0 ) symmetric cross-ply laminated composite plates under sinusoidal loading.

4. Bi-directional bending of three-layer (0 /core/0 ) symmetric sandwich plates under sinusoidal loading.

Displacements and stresses for isotropic, laminated composite and sandwich plates under bi-directional bending obtained by using the present theory (FOSNDT) are presented in Tables 1-4 and compared with those obtained by using the CLPT, the FSDT of Mindlin (1951), HSDT of Reddy (1984), SSNPT of Sayyad and Ghugal (2014b) and exact elasticity solution of Zenkour (2007). The displacements and stresses are calculated at typical important locations using the following non-dimensional form.

  x , y

 b h  uE  a b h  w E  a b h    100

3

3

      u w   0, , ; , , ; x , y , , ;

     

3

4

2

q hS q hS q S  2 2   2 2 2   2 2 2 

(31)

  

 a b z  xy  b z   a z  yz

xz

  

  

, , ; 0, , ; ,0,

xy   xz   yz  

2

 2 2 h  q S  2 h  q S  2 h  q S where S=a/h and E

3 is the elastic modulus of the middle layer.

Example 1: In this example bi-directional bending analysis of isotropic square plate under sinusoidal loading is carried out. Material properties defined by Eq. (28) are used for the numerical study. Displacements and stresses obtained using the present theory are presented in non-dimensional form defined by Eq. (31). Results obtained by using the present theory are compared with exact elasticity solution given by Zenkour (2007) and sinusoidal shear and normal plate theory (SSNPT) of Sayyad and Ghugal (2014b). The results shown in Table 1 reveals that, the present theory accurately predicts the displacements and in-plane normal stresses for thin, moderately thick and thick plates, whereas exact results for in-plane shear stresses are not available in the literature. Transverse shear stresses predicted by the present theory are in excellent agreement with those obtained by using exact elasticity solution.

Example 2: In this example, the present theory is applied for the bending analysis of two-layer (0 /90 ) anti- symmetric laminated composite plates subjected to sinusoidal load. The plate is made up of fibrous composite material defined in Eq. (30). The layers are of equal thickness i.e. /2. The non-dimensional displacements and

h

stresses obtained using the present theory are presented in Table 2 and are compared with classical laminated plate theory (CLPT) of Kirchhoff, first order shear deformation theory (FSDT) of Mindlin (1951), SSNPT of Sayyad and Ghugal (2014b), HSDT of Reddy (1984), and exact elasticity solution given by Zenkour (2007). The examination of Table 2 shows that the transverse displacements obtained by using the present theory are in excellent agreement with exact solution compared to HSDT and SSNPT. This is in fact due to inclusion of transverse normal deformation along with fourth-order variation of transverse displacement. The in-plane



normal stress ( ) predicted by the present theory is also in excellent agreement with exact solution. The

y

present theory yields accurate transverse shear stresses compared to HSDT and SSNPT. This can be considered as a major contribution of the present theory over existing theories. This accuracy of transverse shear stresses is not achieved by other theories such as HSDT of Reddy (1984) and SSNPT of Sayyad and Ghugal (2014b). FSDT and CLPT underestimate the numerical results due to negelect of transverse shear and normal stresses. Through-the- thickness distributions of in-plane displacement, in-plane normal stresses and transverse shear stresses for

/90 laminated composite plates subjected to sinusoidal load are shown in Figs. 2 through 6. The variation of transverse displacement with respect to aspect ratio is shown in Fig. 7.

Example 3: In this example, an efficiency of the present theory is checked for the symmetric laminated laminated composite plates. Three layered (0 /90 /0 ) symmetric laminated composite plate made up of fibrous composite material subjected to sinusoidal load is considered for the numerical study. Material properites are mentioned in Eq. (30). The layers are of equal thickness i.e. h /3. Non-dimensional displacements and stresses are tabulated in Table 3 and the through thickness distributions of in-plane displacement at support, normal stress at mid span and transverse shear stress at boundary edges under the sinusoidal loading are plotted in Figs. 8 through 12. Variation of transverse displacement with respect to aspect ratio is plotted in Fig. 13. The present results are compared with exact solution, CLPT, FSDT, HSDT and SSNPT. It is pointed out from the Table 3 that the transverse displacements and shear stresses obtained by using the present theory are in excellent agreement with exact elasticity solutions. In-plane normal stresses are slightly on higher side compared to other theories available in the literature. FSDT and CLPT underestimate the results.

Example 4: Composite sandwich plates are basically a special form of fibre reinforced composite plates composed of two thin strong, stiff layers (face sheets) which resist bending bonded to a relatively thicker, less dense layer (core) to resist shear force. The validity of the present theory is also checked for the bending analysis of symmetric sandwich plate. A three layered (0 / /90 ) sandwich plate having face sheets of thickness 0.1

core h

each and soft core of thickness 0.8 is considered for the analysis. The material properties of the face sheets are

h

given by Eq. (30) while those for core are given by Eq. (29). Table 4 shows the non-dimensional displacements and stresses. The numerical results obtained by using the present theory are compared with those obtained by SSNPT and exact solution. It is observed that the results obtained by using the present theory are in good agreement with the exact elasticity solution and SSNPT. The through thickness distributions of in-plane displacement, in-plane normal stresses and transverse shear stresses are plotted in Figs. 14 through 18. It is pointed from the distribution that the normal stresses in the core (middle layer) are very less compared to those in face sheets. This is in fact due to high face sheet stiffness to core stiffness ratio. Variation of transverse displacement with aspect ratio is shown in Fig. 19.

Table 1. Non-Dimensional Displacements and Stresses for Isotropic Square Plate

CR CR EE CR EE S Model u w      y   xy xz xz x yz yz

(-h/2) (0) (-h/2) (-h/2) (-h/2) (0) (-h/2) (-h/2) (0)

4 FOSNDT 0.0449 3.6858 0.2132 0.2132 0.1080 0.2765 0.2354 0.2474 0.2354

SSNPT 0.0440 3.653 0.2267 0.2267 0.1063 0.2444 0.2355 0.2424 0.2355

4

• Exact 0.0450 3.6630 0.2040 0.2040 0.2361 0.2361 ---

10 FOSNDT 0.0442 2.9491 0.2005 0.2005 0.1068 0.2770 0.2383 0.2727 0.2383

SSNPT 0.0439 2.9333 0.2125 0.2125 0.1060 0.2454 0.2380 0.2454 0.2380 Exact 0.0443 2.9425 0.1988 0.1988 ---- --- 0.2383 0.2383 ---

20 FOSNDT 0.0441 2.8412 0.1986 0.1986 0.1066 0.2772 0.2387 0.2769 0.2387

SSNPT 0.0439 2.8286 0.2105 0.2105 0.1060 0.2455 0.2384 0.2455 0.2384

Exact ---- ---- --- 0.0440 2.8377 0.1979 0.1979 0.2386 0.2386

50 FOSNDT 0.0441 2.8109 0.1981 0.1981 0.1065 0.2772 0.2388 0.2781 0.2388

SSNPT 0.0439 2.7991 0.2100 0.2100 0.1060 0.2456 0.2385 0.2456 0.2385 Exact 0.0440 2.8082 0.1976 0.1976 --- 0.2386 0.2386 ---- ---

100 FOSNDT 0.0441 2.8066 0.1980 0.1980 0.1065 0.2772 0.2388 0.2783 0.2388

SSNPT 0.0439 2.7949 0.2099 0.2099 0.1060 0.2456 0.2385 0.2456 0.2385

• 0.2387 --- 0.0440 2.8040 0.1976 0.1976 ---- Exact

0.2387 FOSNDT: Present, SSNPT: Sayyad and Ghugal (2014b), Exact: Zenkour (2007) Table 2. Non-Dimensional Displacements and Stresses for (0 /90 ) Laminated Composite Square Plates.

CR CR EE CR EE u w S Model      y   xy xz xz x yz yz

(-h/2) (0) (-h/2) (-h/2) (-h/2) (-h/2) (0) (-h/2) (0)

4 FOSNDT 0.0111 2.0169 0.8960 0.0953 0.0549 0.123 0.116 0.120 0.117

SSNPT 0.0111 1.9424 0.9062 0.0964 0.0562 0.127 0.112 0.127 0.112 HSDT 0.0113 1.9985 0.9060 0.0891 0.0577 0.125 0.110 0.125 0.110 FSDT 0.0088 1.9682 0.7157 0.0843 0.0525 0.091 0.122 0.091 0.122

• CLPT 0.0088 1.0636 0.7157 0.0843 0.0525 0.122 0.122
• Exact 2.0670 0.8410 0.1090 0.0591 0.120 0.125

10 FOSNDT 0.0090 1.2144 0.7398 0.0862 0.0528 0.122 0.121 0.115 0.121

SSNPT 0.0092 1.2089 0.7471 0.0876 0.0530 0.130 0.120 0.130 0.120 HSDT 0.0092 1.2161 0.7468 0.0851 0.0533 0.127 0.120 0.127 0.120 FSDT 0.0088 1.2083 0.7157 0.0843 0.0525 0.091 0.122 0.091 0.122

• CLPT 0.0088 1.0636 0.7157 0.0843 0.0525 0.122 0.122
• Exact 1.2250 0.7302 0.0886 0.0535 0.121 0.125 --- ---

FOSNDT: Present, SSNPT: Sayyad and Ghugal (2014b), HSDT: Reddy (1984), FSDT: Mindlin (1951), CLPT: Kirchhoff (1850), Exact: Zenkour (2007)

0.5 FOSNDT SSNPT

0.25 z/h

• 0.02 -0.01

0.01

0.02

0.03 u

• 0.25
• 0.5

u

Figure 2: Through thickness variation of in-plane displacement ( ) for two-layer (0 /90 ) antisymmetric laminated composite plate subjected to sinusoidal load. (s=4)

0.5 FOSNDT SSNPT z/h

0.25

• 1 -0.5

0.5

1 

x

• 0.25
• 0.5 

Figure 3: Through thickness variation of in-plane normal stress ( x ) for two-layer (0 /90 ) antisymmetric laminated composite plate subjected to sinusoidal load. (s=4)

FOSNDT

0.5

h

SSNPT

z/

0.25

• 1 -0.5

0.5

1

 y

• 0.25
• 0.5



Figure 4: Through thickness variation of in-plane normal stress ( ) for two-layer (0 /90 ) antisymmetric laminated

y

composite plate subjected to sinusoidal load. (s=4)

### 0.5 FOSNDT

SSNPT

0.25

h z/

0.1

0.2

0.3

0.4

 xz

• 0.25
• 0.5



Figure 5: Through thickness variation of transverse shear stress ( ) for two-layer (0 /90 ) antisymmetric laminated

xz

composite plate subjected to sinusoidal load. (s=4)

### 0.5 FOSNDT

SSNPT

0.25

h z/

0.1

0.2

0.3

0.4

 yz

• 0.25
• 0.5



Figure 6: Through thickness variation of transverse shear stress ( yz ) for two-layer (0 /90 ) antisymmetric laminated composite plate subjected to sinusoidal load. (s=4)

5 FOSNDT SSNPT

4

3 w

2

1

20

40

60 80 100 s=a/h w

Figure 7: Variation of transverse displacement ( ) with respect to aspect ratio for two-layer (0 /90 ) antisymmetric laminated composite plate subjected to sinusoidal load.

) for three-layer (0 /90 /0 ) symmetric laminated composite plate subjected to sinusoidal load. (s=4)

4 FOSNDT 0.0100 1.9331 0.8146 0.0846 0.0500 0.1908 0.2653 0.1720 0.2168

SSNPT 0.0092 1.9015 0.7535 0.0880 0.0496 0.2092 0.2768 0.1914 0.2088 HSDT 0.0091 1.9218 0.7345 0.0782 0.0497 0.2024 0.2855 0.1832 0.2086 FSDT 0.0055 1.5681 0.4370 0.0614 0.0369 0.1201 0.3368 0.1301 0.1968 CLPT 0.0068 0.4312 0.5387 0.0267 0.0213 --- 0.3951 --- 0.0823 Exact --- 2.0046 0.7550 0.0949 0.0505 0.2550 --- 0.2170 ---

u

FOSNDT SSNPT Figure 8: Through thickness variation of in-plane displacement (

z/h

0.5

0.25

u

0.01

FOSNDT: Present, SSNPT: Sayyad and Ghugal (2014b), HSDT: Reddy (1984), FSDT: Mindlin (1951), CLPT: Kirchhoff (1850), Exact: Zenkour (2007)

10 FOSNDT 0.0074 0.7305 0.5941 0.0408 0.0285 0.2467 0.3622 0.0958 0.1203

SSNPT 0.0071 0.7155 0.5720 0.0411 0.0278 0.2577 0.3670 0.1070 0.1179 HSDT 0.0071 0.7125 0.5684 0.0387 0.0277 0.2447 0.3693 0.1033 0.1167 FSDT 0.0065 0.6306 0.5134 0.0353 0.0252 0.1363 0.3806 0.0762 0.1108 CLPT 0.0068 0.4312 0.5387 0.0267 0.0213 --- 0.3951 --- 0.0823 Exact --- 0.7528 0.5898 0.0418 0.0289 0.3570 ---- 0.1200 ---

(0)

Table 3. Non-Dimensional Displacements and Stresses for (0 /90 /0 ) Laminated Composite Square Plates.



(-h/2) EE yz



 (0) CR yz

 (-h/2) EE xz

 (-h/2) CR xz

(-h/2) CR xy

(-h/2)

y



S Model u (-h/2) w (0) x

• 0.01 -0.005 0.005
• 0.5
• 0.25

### 0.5 FOSNDT

SSNPT

h z/

0.25

• 1 -0.5

0.5

1

 x

• 0.25
• 0.5



Figure 9: Through thickness variation of in-plane normal stress ( ) for three-layer (0 /90 /0 ) symmetric laminated

x

composite plate subjected to sinusoidal load. (s=4)

### 0.5 FOSNDT

SSNPT

z/h

0.25

• 1 -0.5

0.5

1

 y

• 0.25
• 0.5



Figure 10: Through thickness variation of in-plane normal stress ( ) for three-layer (0 /90 /0 ) symmetric

y

laminated composite plate subjected to sinusoidal load. (s=4)

• 0.5
• 0.25

0.1

yz 

FOSNDT SSNPT Figure 12: Through thickness variation of transverse shear stress (

z/ h

0.5

0.25

 yz

0.25

0.2

0.15

0.05

) for three-layer (0 /90 /0 ) symmetric laminated composite plate subjected to sinusoidal load. (s=4)

xz 

FOSNDT SSNPT Figure 11: Through thickness variation of transverse shear stress (

z/ h

0.5

0.25

 xz

0.3

0.2

0.1

• 0.5
• 0.25

) for three-layer (0 /90 /0 ) symmetric laminated composite plate subjected to sinusoidal load. (s=4)

5 FOSNDT SSNPT

4

3

w

2

1

20

40

60 80 100

s=a/h w

Figure 13: Variation of transverse displacement ( ) with respect to aspect ratio for three-layer (0 /90 /0 ) symmetric laminated composite plate subjected to sinusoidal load.

Table 4. Non-Dimensional Displacements and Stresses for sandwich (0 /core/0 ) Square Plate.

CR CR EE CR EE u w S Model      y   x xy xz xz yz yz

(-h/2) (0) (-h/2) (-h/2) (-h/2) (-h/2) (0) (-h/2) (0)

4 FOSNDT 0.00890 3.599 1.4623 0.2433 0.1392 0.293 0.248 0.111 0.103 SSNPT 0.00858 3.513 1.4313 0.2526 0.1358 0.280 0.243 0.123 0.102 Exact 0.00922 3.798 1.5120 0.2532 0.1430 0.238 0.101 --- ---

10 FOSNDT 0.00690 1.037 1.1355 0.1031 0.0682 0.354 0.303 0.054 0.050 SSNPT 0.00699 1.028 1.1310 0.1089 0.0676 0.345 0.301 0.061 0.050

• Exact 0.00715 1.100 1.1518 0.1098 0.0706 0.299 0.052

20 FOSNDT 0.00690 0.595 1.1048 0.0671 0.0502 0.371 0.318 0.038 0.035 SSNPT 0.00689 0.591 1.1033 0.0715 0.0499 0.363 0.317 0.043 0.035 Exact 0.00695 0.613 1.1096 0.0699 0.0510 0.317 0.036 --- ---

50 FOSNDT 0.00690 0.464 1.0977 0.0555 0.0445 0.377 0.323 0.033 0.030 SSNPT 0.00687 0.462 1.0970 0.0594 0.0443 0.369 0.322 0.037 0.030 Exact 0.00690 0.467 1.0991 0.0569 0.0446 0.323 --- 0.030 --- 100 FOSNDT 0.00690 0.445 1.0967 0.0538 0.0437 0.378 0.324 0.032 0.029

SSNPT 0.00687 0.443 1.0962 0.0576 0.0434 0.369 0.322 0.036 0.030 Exact

• 0.00690 0.446 1.0980 0.0549 0.0436 0.324 --- 0.029

FOSNDT: Present, SSNPT: Sayyad and Ghugal (2014b), Exact: Zenkour (2007)

### 0.5 FOSNDT

h SSNPT z/

0.25

• 0.01 -0.005 0.005

0.01 u

• 0.25
• -0.5

u

Figure 14: Through thickness variation of in-plane displacement ( ) for three-layer (0 /core/0 ) symmetric sandwich plate subjected to sinusoidal load. (s=4)

0.5 FOSNDT SSNPT h z/

0.25

• 1.5 -1 -0.5

0.5

1

1.5 

x

• 0.25
• 0.5 

Figure15: Through thickness variation of in-plane normal stress ( ) for three- layer (0 /core/0 ) symmetric

x

sandwich plate subjected to sinusoidal load. (s=4)

• 0.25 -0.125 0.125
• 0.5
• 0.25

0.15

xz 

Figure 17: Through thickness variation of transverse shear stress (

FOSNDT SSNPT

0.5 z/ h

0.25

0.3  xz

) for three- layer (0 /core/0 ) symmetric sandwich plate subjected to sinusoidal load. (s=4)

y 

FOSNDT SSNPT Figure16: Through thickness variation of in-plane normal stress (

z/h

0.5

0.25

 y

0.25

• 0.5
• 0.25

) for three-layer (0 /core/0 ) symmetric sandwich plate subjected to sinusoidal load. (s=4) FOSNDT SSNPT

0.5

0.25 h z/

0.06

0.12  yz

• 0.25
• 0.5



Figure 18: Through thickness variation of transverse shear stress ( ) for three-layer (0 /core/0 ) symmetric

yz

sandwich plate subjected to sinusoidal load. (s=4)

12 FOSNDT SSNPT

8 w

4

20

40

60 80 100 s=a/h w

Figure 19: Variation of transverse displacement ( ) with respect to aspect ratio for three-layer (0 /core/90 ) symmetric sandwich plate subjected to sinusoidal load.

### 4.0 CONCLUSIONS

A new fifth-order shear and normal deformation theory is developed for the bi-directional bending analysis of laminated composite and sandwich plates subjected to transverse loads. This theory considered the effects of both transverse shear and normal deformations. In-plane and transverse displacements uses a polynomial shape function expanded up to fifth-order in terms of the thickness coordinate to properly account the effects of transverse shear and normal deformations. The present theory does not require a problem dependent shear correction factor as it satisfies traction free boundary conditions at top and bottom surfaces of the plate using constitutive relations. The plate is analysed for simply supported boundary conditions using Navier’s solution technique. From the numerical study and discussion of results it is concluded that the present theory yields accurate prediction of displacements and stresses for all types of laminate configurations compared to other lower and higher order plate theories available in the iterature. The most important contribution of the present theory over existing theories is, it estimates accurate transverse shear stresses for laminated composite and sandwich plates. This accuracy is achieved by including fifth-order variation of displacements and transverse normal deformation. Therefore, it is strongly recommended that, for the accurate analysis of laminated composite and sandwich thick plates, effects of both transverse shear and normal deformations are essential.

References Ambartsumian, S.A. (1958). On the theory of bending plates. Izv Otd Tekh Nauk AN SSSR 5:69–77.

Carrera, E. (1999a). Transverse normal stress effects in multilayered plates. ASME Journal of Applied Mechanics 66(4):1004-1012. Carrera, E. (1999b). A study of transverse normal stress effect on vibration of multilayered plates and shells. Journal of Sound and Vibration 225(5): 803-829. Carrera, E. (2002). Theories and finite elements for multilayered anisotropic, composite plates and shells. Archives of Computational Methods in Engineering 9(2):87-140. Carrera, E. (2003). Theories and finite elements for multilayered anisotropic, composite plates and shells: a unified compact formulation with numerical assessment and benchmarking. Archives of Computational Methods in Engineering 10(3):216-296. Carrera, E., (2005). Transverse normal strain effects on thermal stress analysis of homogeneous and layered plates. AIAA Journal 43(10): 2232-2242. Chakrabarti, A., and Sheikh, A. H. (2005). Analysis of laminated sandwich plates based on interlaminar shear stress continuous plate theory. ASCE Journal of Engineering Mechanics 131(4): 377-384. Ghugal, Y. M., and Sayyad, A. S. (2013). Stress analysis of thick laminated plates using trigonometric shear deformation theory. International Journal of Applied Mechanics 5(1):1–23. Grover, N., Singh, B. N., Maiti, D. K. (2013). Analytical and finite element modeling of laminated composite and sandwich plates: an assessment of a new shear deformation theory for free vibration response. International Journal of Mechanical Science 67:89–99. Kant, T. and Swaminathan, K. (2002). Analytical solutions for the static analysis of laminated composite and sandwich plates besed on a higher order refined theory. Composite Structures 56(4): 329-344. Karama, M., Afaq, K.S., Mistou, S. (2009). A new theory for laminated composite plates. Proceedings of The Institution of Mechanical Engineers, Part L: Journals of Materials: Design and Applications 223:53–62. Kirchhoff, G.R. (1850). Uber das gleichgewicht und die bewegung einer elastischen scheibe. Journal for Pure and Applied Mathematics (Crelle’s Journal) 40:51–88. Levy, M. (1877). Memoire sur la theorie des plaques elastique planes. Journal des Mathematiques Pures et Appliquees 30: 219–306. Mantari, J. L., Oktem, A. S., Soares, C. G. (2012). A new trigonometric shear deformation theory for isotropic, laminated composite and sandwich plates. International Journal of Solids and Structures 49:43–53.